Fabrication and SERS Performance of Silver-Nanoparticle ... yuting/Publications/Publication......
Embed Size (px)
Transcript of Fabrication and SERS Performance of Silver-Nanoparticle ... yuting/Publications/Publication......
Fabrication and SERS Performance of Silver-Nanoparticle-Decorated Si/ZnO Nanotrees in Ordered Arrays Chuanwei Cheng,† Bin Yan,† She Mein Wong,‡ Xianglin Li,† Weiwei Zhou,† Ting Yu,† Zexiang Shen,† Hongyu Yu,‡ and Hong Jin Fan†,*
Division of Physics and Applied Physics, School of Physical and Mathematical Sciences, Nanyang Technological University, 637371 Singapore, and Division of Microelectronics, School of Electrical and Electronic Engineering, Nanyang Technological University, 639798 Singapore
ABSTRACT Highly ordered treelike Si/ZnO hierarchical nanostructures are successfully prepared in a large scale by combining two common techniques, viz., photolithography-assisted wafer-scale fabrication of Si nanopillars and bottom-up hydrothermal growth of ZnO nanorods. Silver nanoparticles are decorated onto the nanotrees by photochemical reduction and deposition. The Si/ZnO/Ag hybrid nanotrees are employed as SERS-active substrates, which exhibit good performance in terms of high sensitivity and good reproducibility. In addition to the SERS application, such ordered Si/ZnO arrays might also find potential applications in light-emitting diodes and solar cells.
KEYWORDS: Si nanowire • ZnO nanorod • hierarchical • hydrothermal, SERS
Rational design and fabrication of hierarchical nano-structures with a tunable dimension and structuralcomplexity have drawn wide attention because of their promising applications in nanoelectronic devices, en- ergy conversion, SERS (surface-enhanced Raman spectros- copy) substrate, and so on (1-5). For example, various groups have reported treelike nanostructures of GaP (6), Zn3P2 (7), PbS (8), and TiO2 (9). Recently we developed a facile method to fabricate tree-like hierarchical nanostruc- tures with ZnO branches on SnO2 backbone nanowires in a large scale by a two-step fabrication process (4).
Since its discovery 30 years ago (10-12), SERS as a powerful high-throughput tool for trace-level molecule detec- tion has stimulated considerable research interest in the scientific community (13-18). In the past few years, much progress has been made in the fabrication of various metal nanostructures as Raman signal enhancing agents (19-23). Recently, it has been demonstrated that using three-dimen- sional (3D) nanostructures as SERS media can dramatically increase the sensitivity (24-30). The 3D nanostructures have advantages of large surface area available for the formation of the so-called “hot spots” (spatially localized surface plasmon resonances between those closely neigh- bored nanoparticles) (31) and the adsorption of target ana- lytes. A number of promising 3D SERS substrates have been proposed, such as porous Si (24) and Al2O3 nanochanels (25),
Si nanotips (26) and nanowires (27), ZnO nanowire arrays (28, 29), and In2P3 nanowire arrays (30).
To bring SERS-based sensor to practical applications, it is desirable that the SERS substrates contain of highly ordered structures with reproducible and controllable ge- ometries. A nanopatterned structure, either 3D or 2D, can provide significant Raman enhancement. A number of techniques are available for 2D patterning of SERS sub- strates, ranging from the conventional electron beam lithog- raphy (32, 33) photolithography (34), to the mordern nano- sphere lithography (35), block copolymer lithography (36, 37), etc. Among these approaches, photolithography has its advantage in terms of large area, high-throughput with relatively low cost, and most importantly, technical compat- ibility with Si industry, which is essential for realizing lab- on-a-chip sensing devices.
In this paper, we fabricated highly ordered treelike Si/ZnO hierarchical nanostructure arrays by combining photolithog- raphy top-down patterning toward ordered Si nanopillar arrays, and subsequent hydrothermal growth of ZnO nano- rods on the Si pillars. The obtained ordered arrays of nanotrees are then coated with Ag nanoparticles in order for SERS applications. Compared to SERS substrates based on nanoparticles films (37) and unidirectional nanowire arrays (26-30), the nanotrees have a much higher specific surface area, thus allowing an increased loading of metal particles and adsorption of a larger number of target molecules, as well as the high possibility of forming 3D plasmon “hot spots”. In addition, it is expected that such ordered patterns can be readily integrated within microfluidic channels and applied in high-throughput screening bioassays.
RESULTS AND DISCUSSION Figure 1 illustrates the fabrication procedure for the 3D
hierarchical SERS substrates. The process mainly involves
* Corresponding author. E-mail: email@example.com. Received for review March 27, 2010 and accepted May 21, 2010 † School of Physical and Mathematical Sciences, Nanyang Technological University. ‡ School of Electrical and Electronic Engineering, Nanyang Technological University. DOI: 10.1021/am100270b
2010 American Chemical Society
A R T IC
1824 VOL. 2 • NO. 7 • 1824–1828 • 2010 www.acsami.org Published on Web 06/01/2010
three steps. First, the patterned Si nanopillar arrays were prepared by standard top-down photolithography followed by dry etching. This step defines the height and interdistance of the trunks. In order to ensure the structure robutness and preserve the patterns, the Si nanopillars herein are relatively thick and short (see below). Subsequently, ZnO branches were grown on the Si nanopillars through a routine hydro- thermal process. The lengths of the nanorods are adustable by controlling the growth time (1-5 h). The ZnO seed layer needed for the hydrothermal growth was coated using atomic layer deposition, which is particularly advantageous in the case of high-aspect-ratio Si pillars. Finally, Ag nano- particles were loaded onto the nanotrees through photo- chemical reduction and deposition.
Figure 2a-d show the top and tilted-view SEM images of the as-prepared Si nanopillar arrays on Si substrate after etching. The pillars are oriented perpendicular to the sub- strate surface with good uniformity. The pillar shows a towerlike morphology with a typical height of 300 nm, the average diameter of Si pillar is about 150 nm and gradually
decreases from the root to the tip. The nearest-neighbor spacing of the pillars is 400 nm, as predefined by shadow mask.
After applying the solution growth of ZnO nanorods, the initially smooth Si pillars branch out, forming tree-like nanostructures. The typical SEM images of such structures are shown in Figure 3a-d. The ZnO nanorod branches are mainly stand perpendicular to the side surfaces of the Si pillars. From the magnified SEM images (Figure 3c,d), the diameter and length of secondary ZnO nanorods are deter- mined to be about 30 nm and 150-200 nm, respectively. The length of ZnO nanorods are controllable by adjusting the growth time (see Figure S1 in the Supporting Informa- tion). Unlike the cases of SnO2 nanowire backbones where the interface epitaxy allows a spacial alignment of the ZnO nanorods (4), the ZnO nanorod branches on the Si pillars are randomly oriented.
Figure 4 shows the representative SEM image of the ordered nanotrees whose branches are decorated with Ag nanoparticles. The metal Ag nanoparticles are successfully deposited onto the surface of both ZnO branches and Si backbones. The diameter of Ag particles is about 20-30 nm. The successful decoation can be more clearlier seen in samples with longer ZnO branches (see the Supporting Information. Figure S2). X-ray diffraction (XRD) analysis was employed to investigate the crystal phase of nanotrees prior to and after the Ag decoration (see the Supporting Informa- tion, Figure S3). The crystal phase of ZnO marked with“∆” is confirmed to be hexagonal wurtzite phase, and the peaks marked with “(” (curve b) can be indexed to face-centered- cubic (fcc) structure of Ag.
To evaluate the SERS activity of the Si/ZnO/Ag nanotree substrates, we measured Raman spectra of R6G molecules adsorbed on three types of different samples: bare Si/ZnO nanotrees, Si/ZnO/Ag nanotrees, and Ag particles on a flat Si surface. The results are depicted in Figure 5. Curve a is from the Si/ZnO nanotrees incubated in 10-5 M R6G solution for 20 min and then washed with deionized water (i.e., without Ag decoration). Only one strong Raman peak located at ∼520 cm-1 is observed, which is assigned to the first- order optical phonon scattering of crystal Si nanopillars and substrate. No R6G related Raman signals can be observed in curve a. For the Si/ZnO/Ag sample (curve c), besides the Si peak, very strong R6G characteristic peaks are present. The Raman bands at 1650, 1570, 1507, 1357, 1310, 1180, 778, and 605 cm-1 are assigned to the xanthene ring stretch, ethylamine group wag, and carbon-oxygenstretch of R6G (38). For comparison, a control Raman study on 2D Ag nanoparticles with diameter of ∼15 nm (see Figure S4 in the Supporting Information for SEM image) on planar Si sub- strate was conducted. As shown in curve b, the Raman enhancement is much weaker than that of the Si/ZnO/Ag nanotree structures. Furthermore, the SERS detection level of R6G molecules for the Si/ZnO/Ag substrates can reach to 1 × 10-9 M (see the Supporting Information, Figure S5).
Quantifying the absolute enhancement factor (EF) is still a matter of debate in literature, which requires accurate data
FIGURE 1. Schematics of the fabrication procedures for the 3D hierarchical SERS substrate, which is ordered Si/ZnO nanotrees decorated by silver nanoparticles.
FIGURE 2. SEM images of the Si nanopillar arrays. (a) Top view and (b) 20° titled view.
A R T IC
www.acsami.org VOL. 2 • NO. 7 • 1824–1828 • 2010 1825